Crystallization of high aspect ratio HKUST-1 thin films in nanoconfined channels for selective small molecule uptake

We present the ability to create unique morphologies of a prototypical metal organic framework (MOF), HKUST-1, by carrying out its crystallization within a set of nano-confined fluidic channels. These channels are fabricated on cyclic olefin copolymer by the high-fidelity hot embossing imprinting method. The picoliter volume synthesis in the nanochannels is hypothesized to bias the balance between nucleation and growth rates to obtain high aspect ratio large-crystalline domains of HKUST-1, which are grown in defined morphologies due to the patterned nanochannels. Confined crystal growth is achieved in nanofluidic channels as shallow as 50 nm. HKUST-1 crystalline domains with aspect ratios greater than 2500, and lengths up to 144 μm are obtained using the nanochannels, exceeding values obtained using chemical modulation and other confinement methods. HKUST-1 crystals are characterized using optical microscopy and scanning electron microscopy with energy dispersive spectroscopy. Porosity of the MOF and selective molecular uptake is demonstrated through inclusion of anthracene and methylene blue within the HKUST-1 framework, and with exclusion of rhodamine B and riboflavin, characterized using a confocal fluorescence microscope. We attribute this selectivity to the analyte size and electrostatic characteristics. Nanoconfined crystallization of MOFs can thus yield control over crystalline morphology to create ideal MOF crystals for enabling selective molecular enrinchment and sensing.


Introduction
Metal-organic frameworks (MOFs) are composed of metal ions or oxo-metallic clusters coordinated with organic linkers. Highly porous, crystalline structures can be created with readily controlled pore geometry and chemistry by changing the metallic cluster or the organic linker. 1,2 Due to their structural and chemical tunability, MOFs are useful for chemical storage, separations, electronic and photonic devices, catalysis, and many other applications. [3][4][5][6][7] Several MOFs have been employed as molecular sieves to selectively enrich small molecules. [8][9][10] Selective enrichment can be coupled with electrical or optical sensing techniques for detection of small molecules at low concentrations. 11,12 The selectivity, enrichment and response time of MOF-based sensors are dependent on the analyte diffusion properties within the MOF. A variety of interactions can be utilized to inuence adsorbate or analyte uptake and transport. For example, the adsorption capacity of the MOF MIL-101 for methyl orange, an anionic dye, was found to be enhanced by increasing the positive charge present on the MOF. 13 MOF crystals with large aspect ratios and lowered defect concentrations have been shown to enhance charge and mass transport. 14,15 Interaction between the guest molecule and the MOF can also be regulated by varying the MOF morphology. For example, a high aspect ratio MOF crystal can allow for selectivity due to predominating crystal facets that are accessible to the guest molecule (e.g. the {111} and {100} planes feature different electrostatic and chemical functionality that impacts analyte diffusion). 16 Currently, MOF morphologies with large aspect ratios are not easily synthesized using bulk synthetic techniques. It is typical to control morphology through pre-or post-synthetic modications (e.g. addition of surface directing agents). [17][18][19] Several groups have utilized conned crystallization to control nucleation and growth of multiple material systems (including small organic molecules, perovskites and MOFs). [20][21][22] The reduced volumes and small working dimensions in conned systems allow for precise regulation of heat and mass transport to modulate conditions during MOF formation. 20 Recent approaches to conned crystallization in MOFs include interfacial synthesis and diffusion-mediated growth, providing control over MOF aspect ratio and creating oriented MOF thin lms. [21][22][23] Microstamping was used by Ameloot et al. to create nano-sized HKUST-1 single crystals in controlled patterns. 24 Previous work has achieved MOF synthesis (ZIF-8, with aspect ratio 60) by growing nano-conned crystals inside anodized aluminum oxide or track etched polycarbonate membranes. 25 Additionally, MOF nanosheets with aspect ratios of 1000 were formed using a biphasic synthesis method. 26 A technique termed solution shearing can promote self-conned thin lm growth in numerous organic molecules. [27][28][29] Connement based growth was also achieved by altering the wetting properties of a substrate to grow oriented, single crystals of an organic semiconductor, C8-BTBT. 30 Perovskite single crystal domains were formed using ink transfer technology for geometric connement during synthesis. 31 Building from previous connement techniques and applying nanouidic crystallization technology to MOFs, the work presented here demonstrates the utility of nanochannel connement-based crystallization to create high aspect ratio MOF crystals. In addition to improving MOF morphology control during synthesis, this study aims to lay the groundwork for nanouidic small molecule enrichment using high aspect ratio MOFs.
We report a parallelized nanouidic platform, fabricated via a hot-embossing nano imprint lithography method (HE NIL), for conned MOF crystal nucleation and growth. HE NIL can reliably replicate the nanoscale features of a master mold in an inexpensive wafer made of thermoplastic cyclic olen copolymer (COC). We show that nano-connement can aid in producing high aspect ratio, crystalline domains of a prototypical MOF, HKUST-1. Using an evaporation driven synthesis, HKUST-1 nucleation and growth occurs along the nanochannel length to yield high aspect ratio crystals. We observed crystal formation with aspect ratios up to 2500, exceeding that of any other previously reported MOFs to the best of the authors' knowledge. 32,33 Finally, the capacity for selective molecular uptake and exclusion in high aspect ratio HKUST-1 crystals is demonstrated using anthracene, methylene blue, rhodamine B and riboavin.

Results and discussion
Nanochannel fabrication and conned crystallization Closed nanochannel arrays are created by the hot embossed bonding of two cyclic olen copolymer (COC) substrates. The bottom substrate is patterned with nanochannel features that are transferred from a so stamp embossing process (ESI Fig. 1 †). The top COC plate contains microuidic through-holes to serve as uid inlet and outlets surrounding the enclosed channels ( Fig. 1, ESI Fig. 2 †).
Each nanochannel array contains a potential loading volume on the order of picoliters per nanochannel, and each array contains 50-100 channels. Channels with widths 0.5-5 mm, depths 60-350 nm, and lengths 2-5 mm were used in this study (ESI Tables 1 and 2 †).
The nanochannels were loaded by placing a small volume of HKUST-1 precursor solution (5 mL) in the channel ports. Capillary action was observed to wick solution from the inlets, lling the void space in the empty channels. Using this technique most channels show ll efficiencies ranging from 40-70% (ESI Fig. 3 †). Crystallization in the nanochannels is induced via solvent evaporation through a combination of vacuum application and heating.
As solvent evaporates from the channels, the solution front recedes at a rate of roughly 0.5 mm h À1 , measured by observing the moving air-liquid interface from optical micrographs. The evaporation rate of solvent is slower than the diffusion rate of the precursors, therefore the spatial concentration of MOF precursor materials can be approximated to be uniform throughout the length of the channel. 34 We hypothesize that during crystallization the concentration increase of the metal ion and the organic linker in the solution is uniform throughout the channel length, and heterogeneous HKUST-1 nucleation occurs throughout the length of the channel, rather than preferentially at the air-liquid interface. However, crystallization also occurs in clusters spanning several channels, suggesting that defects or localized surface properties of the nanochannels may promote nucleation.
Nanouidic crystallization is able to reduce the occurrence of multiple nucleation events compared to bulk synthetic techniques, due to the reduced volumes available per nanochannel for crystallization. 35 The decreased number of nucleation events, coupled with slow growth of the MOF crystal, produces large, high aspect ratio crystals that are shaped by the channel dimensions over the course of several days.

Morphology and characterization of nanoconned HKUST-1 crystals
Bulk HKUST-1, like many other MOFs, is known to have faceted crystal shapes under ideal growth conditions. 16 As the crystals grow, surface energy minimization causes the crystal to exhibit different morphologies. Smaller crystals with square faces (associated with the {100} crystal plane) eventually grow into more stable structures with different faceting (e.g. the hexagonal or triangular {111} planes). 36 In conned nanouidic growth, similar faceting is observed and diverse morphologies of crystals in the nanouidic channels are observed during the growth process (Fig. 2). Observing the population of HKUST-1 crystals that did not grow to ll the channel width, both hexagonal and square prism shaped crystals nucleate in the nanochannels (ESI Fig. 4 †). HKUST-1 crystals that grow in the hexagonal shape indicate that the {111} plane is oriented with respect to the nanochannel width, while the square prism shape indicates that the {100} plane is oriented with respect to the nanochannel width. This result agrees with other reported equilibrium morphologies found in thin lm and conned HKUST-1, where channel surface chemistry and facet-channel interaction can inuence the orientation and morphology of crystals (ESI Fig. 5 †). 16,24,37 Faceting is observed on the crystal edges, and we hypothesize that facets correspond to the slow-growing planes associated with the equilibrium HKUST-1 crystal morphology. 16 As growth proceeds, we hypothesize that the crystal growth is rst conned by the nanochannel height (60-350 nm) and then conned by the nanochannel width (0.5-5 mm), depending on the geometry of each channel ( Fig. 2a and b). Following these connement events, crystal growth occurs along the length of the channel (Fig. 2c). This mode of crystalline growth allows HKUST-1 crystal length to greatly exceed the depth (Fig. 2d).
Assessing the aspect ratio, dened as the ratio of crystal length to depth, we observe that the channels with the shallowest depths (30 nm) produce the largest aspect ratio (ESI Table 3 †). The highest aspect ratio observed in this study was approximately 2500 (ESI Fig. 6 †), an improvement on previously reported results. 33,38 Conversely, the larger depth channels ($300 nm) produce aspect ratios on the order of 200. This nding suggests that depth connement was signicant to producing the highest aspect ratio MOF crystals. The role of channel width on crystallization warrants additional study. However, results suggest that the width dimension does not need to be conned to the same degree as depth (100 nm or less), as widths in the 0.5-1 mm range yield aspect ratios greater than 1000. This is signicant, as making and lling channels becomes more difficult as both the depth and width become smaller; hence wider channels that are easier to load with uid and with nanoconnement in depth alone are sufficient to form high aspect ratio crystals.
The material properties of the obtained crystals are also consistent with the expected properties of HKUST-1. The nal crystallized material is insoluble in ethanol, while the starting materials, trimesic acid and copper nitrate, are soluble. Hence, upon washing the nanochannels aer crystallization, the remaining crystal has a thin lm morphology and solvent compatibility consistent with that of HKUST-1.
Energy dispersive X-ray spectroscopy (EDS) was used to examine the elemental constituents of the crystals in the nanochannels, providing further evidence of HKUST-1. Fig. 3a demonstrates colocalization of copper, carbon and oxygen within the crystal. A decrease in carbon signature of the MOF relative to the COC (a carbon-based polymer) substrate differentiates the HKUST-1 crystals and the nanochannels.  The nitrogen signal remains at noise level, while a copper nitrate control shows appreciable nitrogen signal (ESI Fig. 7 †). Therefore, EDS results suggest that copper and nitrate ions from the Cu(NO 3 ) 2 hydrate precursor dissociate. The presence of the oxygen signature in the crystal, combined with the absence of the nitrogen signature, indicates that the copper is likely coordinating with the trimesic acid linker. Furthermore, the elemental signatures in the nanoconned HKUST-1 are consistent with the signals obtained from bulk HKUST-1 control EDS scan (Fig. 3b). Conventional characterization techniques such as BET-based surface area analysis, TEM and X-ray diffraction prove infeasible due to the small amount of material and the sensitivity of the crystals to the degradation using these characterization techniques.
To probe the crystallinity of the HKUST-1 in the nanochannels, cross sections of the nanochannels were prepared for transmission electron microscopy (TEM) using a focused ion beam (FIB), but TEM diffraction does not conclusively yield a pattern representative of HKUST-1 or its precursors. We hypothesize that the FIB process is destructive to the HKUST-1, and can back-deposit organic material into the porous structure (ESI Fig. 8 †). 39 A bulk HKUST-1 crystal subjected to the same FIB/TEM procedure also degrades similarly. More work is required to overcome challenges associated with high energy characterization techniques to develop full understanding of the single-crystal behaviour in nanoconned environments for this system.

Loading small molecules into high aspect ratio HKUST-1 crystals
Aer removing the top layer of COC to expose the crystals and nanochannels, pure ethanol was used to wash away unreacted material and debris loosely present on the surface. Despite challenges in characterization, the functional utility of the porous MOF is demonstrated through the capacity of the crystals to uptake and exclude different molecular species. HKUST-1 has two pore apertures of 10Å and 14Å. Four different uorescently active molecules were selected as candidate guest molecules. These molecules were selected because they have similar conjugated cores, with anthracene being the simplest, containing three aromatic rings. The other molecules have larger molecular size and greater chemical complexity due to the introduction of additional functional groups or charges (Fig. 4).
To determine if the guest molecules can enter HKUST-1 selectively, anthracene, methylene blue, riboavin or rhodamine B were dissolved in ethanol at their saturation concentration at room temperature. The nanochannels were then immersed in the prepared solution and le overnight to allow sufficient time for diffusion to occur before imaging, although diffusion in MOFs has been shown to occur within minutes. 40 Fig. 4 summarizes the results of molecular inclusion of methylene blue and anthracene, with the exclusion of rhodamine B and riboavin.
Previous studies have shown that the MOF ZIF-8 can be loaded with anthracene while still preserving the characteristic uorescent emission of anthracene. 41 We observed that anthracene can also penetrate the framework of HKUST-1 (Fig. 4a). The presence of anthracene seems to have little effect on the appearance of the HKUST-1 crystal; the brighteld image of the anthracene loaded HKUST-1 does not show any signicant change. The methylene blue loaded HKUST-1 (Fig. 4b) appears much darker in the brighteld image, showing that there is decreased light transmission through the methylene blue loaded HKUST-1 crystals.
The dark blue color of methylene blue allows for bright-eld optical characterization (ESI Fig. 9 †) while the uorescence allows for sensitive measurements to be made while minimizing signal from the COC and HKUST-1. Both techniques show that methylene blue is located inside the crystal, indicating that the formation of a high aspect ratio and porous HKUST-1 crystal was achieved in the nanochannels (Fig. 4b). The capacity for a MOF to uptake these materials is not unique; previous reports have demonstrated methylene blue diffusion into the pores of HKUST-1. 42,43 However, the advantage of nanoconned MOF crystallization is the potential for localized and selective enrichment of analytes to enhance detection selectivity.
The nanoconned diffusion path length from the top to the bottom of the channel allows for rapid equilibration of the analytes with minimal concentration gradient across the channel depth. The uniformity of the thin lm and the large aspect ratios also allows for clear optical or uorescent detection of analytes due to the uniform optical path length (Fig. 4, ESI Fig. 10 †). Fig. 4c shows that rhodamine did not enter the MOF at a detectable concentration. The signal in the image is from small crystallites of rhodamine B deposited on the channel surface, or is noise during the imaging. Finally, riboavin is not detected within the HKUST-1 crystals either. The images in Fig. 4d show a large crystal, which is hypothesized to be ribo-avin that was deposited as ethanol evaporated during the drying process, causing riboavin to precipitate out of solution. Therefore, the porous MOF has the ability to be used for small organic molecule separations (e.g. allowing methylene blue to pass through the crystal while keeping rhodamine B out) 44 Through this, the utility of high aspect ratio nanochannel crystallization of a MOF is made clear. It can serve as a platform for capture and enrichment of a material, followed by subsequent detection. This is feasible even when there is only a small amount of material available, such as for biomarker detection, which requires sensitivity and specicity for detection, despite limitations of small working volumes. 45,46 Additional studies for crystallization were performed in the nanoconned channels using the precursor for methyl ammonium lead iodide (MAPbI 3 ), a perovskite structure frequently used for solar cell applications. While conned crystallization did occur within the nanochannels (ESI Fig. 11 †), the optimal concentration and crystallization conditions required to achieve high aspect ratio and single crystalline growth are still being explored.

Conclusion
We present the rst report on crystallization of HKUST-1 in parallel arrays of nanoconned channels for studying crystal morphology and characterizing the crystals for selective uptake of small organic molecules. Crystal morphology, porosity, elemental mapping and uorescence microscopy techniques indicate that oriented, high aspect ratio, crystalline domains of HKUST-1 were formed in nanochannels. Moreover, aspect ratios greater than those previously reported for MOFs were obtained, reaching 2500. This work provides the foundation for a range of fundamental studies involving MOFs and other two component reaction-crystallization systems with applications in understanding thin lm growth, nucleation and growth, diffusion kinetics, and in sensing guest molecules in MOFs.
With a well-dened and optically accessible growth region, we are able to observe the nucleation and growth of individual HKUST-1 crystals using readily available optical techniques. Future studies will focus on controlling and understanding crystallization kinetics for tunable crystal aspect ratios. By adjusting concentration and temperature, it is possible to bias a system towards nucleation or growth dominated regimes. 47,48 The nanouidic device studied here can be further developed with patterning and dynamic ow control for increased control over crystal growth direction and morphology.
Large crystal domains of HKUST-1 allow for lower impact of grain boundaries for highly efficient sensing and separation. In future work, uid ow can also be introduced into the nanochannels aer the creation of high aspect ratio MOF crystals to achieve spatial and temporal control over the introduction of guest molecules (analytes).
There is a rich eld of future work possible with this technology, as the platform is ideal for integration with many applications (including sensing and separations). We intend to study the diffusion of small uorescent molecules out of the HKUST-1 crystal in the nanochannels. This is important for probing the mechanism of diffusion in MOF materials, related to zeolites and other mesoporous materials where surface interactions are signicant for material performance. This work will be extended in the future to molecular biomarkers that are usually present at dilute levels within biouids prior to signicant disease progression, thereby requiring signicant levels of enrichment before detection may be possible. 49 In this context, MOFs designed for selectivity to particular molecules and synthesized within a nanoconned platform to form high aspect ratio, defect-free crystals, can be coupled to a micro-uidics network to enable selective analyte enrichment and detection. Finally, separations and sensing applications can leverage the high aspect ratio and nanometer thickness of the crystals grown in this study.
Nanochannel fabrication and materials. Silicon wafers (University Wafer) were patterned by electron beam lithography and reactive ion etching to fabricate a master mold containing a network of nanochannels connected to microchannels. 45,50 This master mold was used to fabricate nanochannels by hot emboss imprinting on 175 mm thickness cyclic olen copolymer or COC substrates (Microuidic-Chip Shop: TOPAS), by using a working stamp polymer M7+IGRACURE 2022 (EV group, Inc.) as an intermediary stamp to prevent damage to the master mold. 51 The nanochannels were then bonded to a 175 mm thick COC cover slip (Microuidic-Chip Shop: TOPAS), which was drilled for inlet and outlet reservoirs that lead to the micro-uidic channels.

Methods
HKUST-1 crystallization. Precursor solution was prepared with Cu(NO 3 ) 2 $2.5H 2 O, trimesic acid and DMSO following the general procedure outlined by Ameloot et al. 24 A typical precursor was made by completely dissolving 1.22 g Cu(NO 3 ) 2 -$2.5H 2 O in 5 mL of DMSO, then dissolving 0.58 g of trimesic acid in the same solution. The nal solution volume was 5.625 mL, yielding metal and linker concentrations of 0.93 M and 0.49 M, respectively. Channels were loaded by placing a small quantity (5 mL) of the precursor solution on the channel ports. Capillary action was observed to wick precursor into the nanochannels immediately aer placement. Excess uid at channel ports was gently removed using a Kimwipe. Channels were imaged aer loading to determine initial loading efficiency. HKUST-1 crystallization was induced by evaporating solvent from the channels. A vacuum oven could be used to control the pressure to increase evaporation rate and enhance crystallization.
Fluorescent molecule loading. To study molecular uptake in the HKUST-1 crystals, nanochannels containing crystals were immersed in a solution of pure ethanol and a uorophore (either anthracene, methylene blue, rhodamine B or riboavin). These solutions were prepared at saturation concentration. The channels with crystals soaked in this solution for 24 hours. To allow sufficient time for the molecule to penetrate the MOF framework and ll the pores. The channels were briey rinsed with ethanol, dried in ambient conditions, and imaged using a confocal microscope.
Crystal characterization. A Zeiss Scope A.1 optical microscope with an Axiocam 503 Color camera was used to image crystals within the nanochannels. A Zeiss 780 NLO confocal laser scanning microscope was used for uorescence imaging of crystals aer soaking with the uorescent molecules. The uorescence was measured using an external transmission NDD PMT detector.
A Quanta 650 scanning electron microscope (SEM) (5 kV, spot size 4, Everhart-Thornley detector) was used to collect morphological data from crystals in the nanochannels. Energy dispersive X-ray spectroscopy (EDS) (18 kV beam, Oxford Instruments, X-Max N 80) was used analyze elemental composition of crystals in delaminated channels. Channels were prepared for these processes by sputter coating them with a protective layer ($20 nm thick) of gold-palladium using a Precision Etching and Coating System (Model 682 PECS).

Conflicts of interest
The authors declare no conicts.